LMucko/crystallography-open-database huggingface dataset:
An electron diffraction study of thin films of cuprous iodide
Kurdyumova, R.N.; Baranova, R.V.; Kristallografiya 6 (1961) 402–405; doi:

data_1542227
_publ_section_title
;
 An electron diffraction study of thin films of cuprous iodide
;
_journal_name_full               Kristallografiya
_journal_page_first              402
_journal_page_last               405
_journal_volume                  6
_journal_year                    1961
_chemical_formula_sum            'Cu I'
_space_group_IT_number           156
_symmetry_space_group_name_Hall  'P 3 -2"'
_symmetry_space_group_name_H-M   'P 3 m 1'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   4.25
_cell_length_b                   4.25
_cell_length_c                   20.86
_cell_volume                     326.304
_citation_journal_id_ASTM        KRISAJ
_cod_data_source_file            Kurdyumova_KRISAJ_1961_1682.cif
_cod_data_source_block           Cu1I1
_cod_original_cell_volume        326.3043
_cod_original_formula_sum        'Cu1 I1'
_cod_database_code               1542227
The Crystal Structures of Ni O (Ba O)3, Ni O Ba O, Ba Ni O3, and Intermediate Phases With Composition Near Ba2 Ni2 O5, with a Note on Ni O
Lander, J.J.; Acta Crystallographica (1,1948-23,1967) 4 (1951) 148–156; doi:

data_2311077
_publ_section_title
;
 The Crystal Structures of Ni O (Ba O)3, Ni O Ba O, Ba Ni O3, and
 Intermediate Phases With Composition Near Ba2 Ni2 O5, with a Note on Ni O
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              148
_journal_page_last               156
_journal_volume                  4
_journal_year                    1951
_chemical_formula_sum            'Ba Ni O2'
_chemical_name_systematic        'Ni Ba O2'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.73
_cell_length_b                   9.2
_cell_length_c                   4.73
_cell_volume                     249.347
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Lander_ACCRA9_1951_1817.cif
_cod_data_source_block           Ba1Ni1O2
_cod_original_cell_volume        249.3467
_cod_original_formula_sum        'Ba1 Ni1 O2'
_cod_database_code               2311077
The crystal structures of Ni O (Ba O)3, Ni O Ba O, Ba Ni O3, and intermediate phases with composition near Ba2 Ni2 O5, with a note on Ni O
Lander, J.J.; Acta Crystallographica (1,1948-23,1967) 4 (1951) 148–156; doi:

data_2311078
_publ_section_title
;
 The crystal structures of Ni O (Ba O)3, Ni O Ba O, Ba Ni O3, and
 intermediate phases with composition near Ba2 Ni2 O5, with a note on Ni O
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              148
_journal_page_last               156
_journal_volume                  4
_journal_year                    1951
_chemical_formula_sum            'Ba3 Ni O4'
_chemical_name_systematic        'Ni Ba3 O4'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-P 3* 2n'
_symmetry_space_group_name_H-M   'R -3 c :R'
_cell_angle_alpha                66.8
_cell_angle_beta                 66.8
_cell_angle_gamma                66.8
_cell_formula_units_Z            2
_cell_length_a                   7.14
_cell_length_b                   7.14
_cell_length_c                   7.14
_cell_volume                     294.970
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Lander_ACCRA9_1951_1818.cif
_cod_data_source_block           Ba3Ni1O4
_cod_original_cell_volume        294.9705
_cod_original_sg_symbol_Hall     '-R 3 2"c (-y+z,x+z,-x+y+z)'
_cod_original_formula_sum        'Ba3 Ni1 O4'
_cod_database_code               2311078
The crystal structure of ammonium hexasulphitoferrate(III), (N H4)9 (Fe (S O)6)
Larsson, L.O.; Niinisto, L.; Acta Chemica Scandinavica (1-27,1973-42,1988) 27 (1973) 859–867; doi:

data_1542228
_publ_section_title
;
 The crystal structure of ammonium hexasulphitoferrate(III), (N H4)9 (Fe
 (S O)6)
;
_journal_name_full               'Acta Chemica Scandinavica (1-27,1973-42,1988)'
_journal_page_first              859
_journal_page_last               867
_journal_volume                  27
_journal_year                    1973
_chemical_formula_sum            'Fe H36 N9 O18 S6'
_chemical_name_systematic        '(N H4)9 (Fe (S O3)6)'
_space_group_IT_number           147
_symmetry_space_group_name_Hall  '-P 3'
_symmetry_space_group_name_H-M   'P -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   10.2226
_cell_length_b                   10.2226
_cell_length_c                   7.2055
_cell_volume                     652.105
_citation_journal_id_ASTM        ACSAA4
_cod_data_source_file            Larsson_ACSAA4_1973_1041.cif
_cod_data_source_block           H36Fe1N9O18S6
_cod_original_cell_volume        652.1049
_cod_original_formula_sum        'H36 Fe1 N9 O18 S6'
_cod_database_code               1542228
Crystal structure and phase transformations of sodium diarsenate, Na4 As2 O7
Leung, K.Y.; Calvo, C.; Canadian Journal of Chemistry 51 (1973) 2082–2088; doi:

data_1542229
_publ_section_title
;
 Crystal structure and phase transformations of sodium diarsenate, Na4 As2
 O7
;
_journal_name_full               'Canadian Journal of Chemistry'
_journal_page_first              2082
_journal_page_last               2088
_journal_volume                  51
_journal_year                    1973
_chemical_formula_sum            'As2 Na4 O7'
_chemical_name_systematic        'Na4 (As2 O7)'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 92.87
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.969
_cell_length_b                   10.126
_cell_length_c                   12.272
_cell_volume                     740.815
_citation_journal_id_ASTM        CJCHAG
_cod_data_source_file            Leung_CJCHAG_1973_998.cif
_cod_data_source_block           As2Na4O7
_cod_original_cell_volume        740.8151
_cod_database_code               1542229
Structures of the Re O3 - type with Reccurent Dislocations of Atoms: 'Homologous Series' of Molybdenum and Tungsten Oxides
Magneli, A.; Acta Crystallographica (1,1948-23,1967) 6 (1953) 495–500; doi:

data_2311079
_publ_section_title
;
 Structures of the Re O3 - type with Reccurent Dislocations of Atoms:
 'Homologous Series' of Molybdenum and Tungsten Oxides
;
_journal_name_full               'Acta Crystallographica (1,1948-23,1967)'
_journal_page_first              495
_journal_page_last               500
_journal_volume                  6
_journal_year                    1953
_chemical_formula_sum            W10
_chemical_name_systematic        'W10 O29'
_space_group_IT_number           10
_symmetry_space_group_name_Hall  '-P 2y'
_symmetry_space_group_name_H-M   'P 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 85.28
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   12.05
_cell_length_b                   3.767
_cell_length_c                   23.59
_cell_volume                     1067.174
_citation_journal_id_ASTM        ACCRA9
_cod_data_source_file            Magneli_ACCRA9_1953_27.cif
_cod_data_source_block           W10
_cod_database_code               2311079
Preparation and structure of La Co8 P5
Meisen, U.; Jeitschko, W.; Zeitschrift fuer Kristallographie (149,1979-) 167 (1984) 135–143; doi:

data_8104505
_publ_section_title
;
 Preparation and structure of La Co8 P5
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              135
_journal_page_last               143
_journal_volume                  167
_journal_year                    1984
_chemical_formula_sum            'Co8 La P5'
_chemical_name_systematic        'La Co8 P5'
_space_group_IT_number           59
_symmetry_space_group_name_Hall  '-P 2ab 2a'
_symmetry_space_group_name_H-M   'P m m n :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.501
_cell_length_b                   3.596
_cell_length_c                   9.342
_cell_volume                     352.769
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Meisen_ZEKRDZ_1984_1829.cif
_cod_data_source_block           Co8La1P5
_cod_original_cell_volume        352.7688
_cod_original_formula_sum        'Co8 La1 P5'
_cod_database_code               8104505
The Crystal Structures of Pb O Pb X O4 (X = S, Cr, Mo) at 5 K by Neutron Powder Profile Refinement
Mentzen, B.F.; Latrach, A.; Bouix, J.; Hewat, A.W.; Materials Research Bulletin 19 (1984) 549–554; doi:

data_1542230
_publ_section_title
;
 The Crystal Structures of Pb O Pb X O4 (X = S, Cr, Mo) at 5 K by Neutron
 Powder Profile Refinement
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              549
_journal_page_last               554
_journal_volume                  19
_journal_year                    1984
_chemical_formula_sum            'O5 Pb2 S'
_chemical_name_systematic        '(Pb O) (Pb (S O4))'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.885
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   13.7576
_cell_length_b                   5.6578
_cell_length_c                   7.0322
_cell_volume                     492.454
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Mentzen_MRBUAC_1984_1255.cif
_cod_data_source_block           O5Pb2S1
_cod_original_cell_volume        492.4541
_cod_original_formula_sum        'O5 Pb2 S1'
_cod_database_code               1542230
The crystal structures of Pb O Pb X O4 (X = S, Cr, Mo) at 5 K by neutron powder profile refinement
Mentzen, B.F.; Latrach, A.; Bouix, J.; Hewat, A.W.; Materials Research Bulletin 19 (1984) 549–554; doi:

data_1542231
_publ_section_title
;
 The crystal structures of Pb O Pb X O4 (X = S, Cr, Mo) at 5 K by neutron
 powder profile refinement
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              549
_journal_page_last               554
_journal_volume                  19
_journal_year                    1984
_chemical_formula_sum            'Cr O5 Pb2'
_chemical_name_systematic        '(Pb O) (Pb (Cr O4))'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 115.33
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.0076
_cell_length_b                   5.6445
_cell_length_c                   7.1028
_cell_volume                     507.597
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Mentzen_MRBUAC_1984_1256.cif
_cod_data_source_block           Cr1O5Pb2
_cod_original_cell_volume        507.5973
_cod_original_formula_sum        'Cr1 O5 Pb2'
_cod_database_code               1542231
The Crystal Structures of Pb O Pb X O4 (X = S, Cr, Mo) at 5 K by Neutron Powder Profile Refinement
Mentzen, B.F.; Hewat, A.W.; Latrach, A.; Bouix, J.; Materials Research Bulletin 19 (1984) 549–554; doi:

data_1542232
_publ_section_title
;
 The Crystal Structures of Pb O Pb X O4 (X = S, Cr, Mo) at 5 K by Neutron
 Powder Profile Refinement
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              549
_journal_page_last               554
_journal_volume                  19
_journal_year                    1984
_chemical_formula_sum            'Mo O5 Pb2'
_chemical_name_systematic        'Pb2 O (Mo O4)'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 114.286
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.2058
_cell_length_b                   5.7592
_cell_length_c                   7.2844
_cell_volume                     543.225
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Mentzen_MRBUAC_1984_1258.cif
_cod_data_source_block           Mo1O5Pb2
_cod_original_cell_volume        543.2255
_cod_original_formula_sum        'Mo1 O5 Pb2'
_cod_database_code               1542232
Structure cristalline de la phase haute temperature de Pb S O4 * 2 Pb O a 973K
Mentzen, B.F.; Latrach, A.; Garnier, P.; Boher, P.; Bouix, J.; Materials Research Bulletin 19 (1984) 925–934; doi:

data_1542233
_publ_section_title
;
 Structure cristalline de la phase haute temperature de Pb S O4 * 2 Pb O a
 973K
;
_journal_name_full               'Materials Research Bulletin'
_journal_page_first              925
_journal_page_last               934
_journal_volume                  19
_journal_year                    1984
_chemical_formula_sum            'O6 Pb3 S'
_chemical_name_systematic        'Pb S O4 (Pb O)2'
_space_group_IT_number           11
_symmetry_space_group_name_Hall  '-P 2yb'
_symmetry_space_group_name_H-M   'P 1 21/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 102.395
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   7.1816
_cell_length_b                   5.7848
_cell_length_c                   8.0528
_cell_volume                     326.749
_citation_journal_id_ASTM        MRBUAC
_cod_data_source_file            Mentzen_MRBUAC_1984_1839.cif
_cod_data_source_block           O6Pb3S1
_cod_original_cell_volume        326.7486
_cod_original_formula_sum        'O6 Pb3 S1'
_cod_database_code               1542233
Preparation et etude de Li2 Ni O3-y (y <= 0.135)
Migeon, H.N.; Courtois, A.; Gleitzer, C.; Zanne, M.; Revue de Chimie Minerale 13 (1976) 1–8; doi:

data_1542234
_publ_section_title
;
 Preparation et etude de Li2 Ni O3-y (y <= 0.135)
;
_journal_name_full               'Revue de Chimie Minerale'
_journal_page_first              1
_journal_page_last               8
_journal_volume                  13
_journal_year                    1976
_chemical_formula_sum            'Li2 Ni O2.88'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 99.85
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   4.884
_cell_length_b                   8.463
_cell_length_c                   9.495
_cell_volume                     386.674
_citation_journal_id_ASTM        RVCMA8
_cod_data_source_file            Migeon_RVCMA8_1976_1287.cif
_cod_data_source_block           Li2Ni1O2.88
_cod_original_cell_volume        386.6743
_cod_original_formula_sum        'Li2 Ni1 O2.88'
_cod_database_code               1542234
Crystal Structure of Para-enriched Solid Deuterium Below the lambda Transition
Mucker, K.F.; White, D.; Talhouk, S.; Harris, P.M.; Physical Review Letters 16 (1966) 799–801; doi:

data_1542235
_publ_section_title
;
 Crystal Structure of Para-enriched Solid Deuterium Below the lambda
 Transition
;
_journal_name_full               'Physical Review Letters'
_journal_page_first              799
_journal_page_last               801
_journal_volume                  16
_journal_year                    1966
_chemical_formula_sum            D
_space_group_IT_number           205
_symmetry_space_group_name_Hall  '-P 2ac 2ab 3'
_symmetry_space_group_name_H-M   'P a -3'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   5.084
_cell_length_b                   5.084
_cell_length_c                   5.084
_cell_volume                     131.406
_citation_journal_id_ASTM        PRLTAO
_cod_data_source_file            Mucker_PRLTAO_1966_649.cif
_cod_data_source_block           D2
_cod_depositor_comments
;

2024-06-03
Z value and formula fixed to values more according to usual
chemical conventions.                 miguel
;
_cod_original_formula_sum            D2
_cod_original_formula_units_Z            2
_cod_original_cell_volume        131.4064
_cod_database_code               1542235
X-ray studies on protoenstatite II. Effect of temperature on the structure up to near the incongruent melting point
Murakami, T.; Takeuchi, Y.; Yamanaka, T.; Zeitschrift fuer Kristallographie (149,1979-) 166 (1984) 263–275; doi:

data_8104506
_publ_section_title
;
 X-ray studies on protoenstatite II. Effect of temperature on the
 structure up to near the incongruent melting point
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              263
_journal_page_last               275
_journal_volume                  166
_journal_year                    1984
_chemical_formula_sum            'Mg O3 Si'
_chemical_name_systematic        'Mg (Si O3)'
_space_group_IT_number           60
_symmetry_space_group_name_Hall  '-P 2n 2ab'
_symmetry_space_group_name_H-M   'P b c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   9.349
_cell_length_b                   8.929
_cell_length_c                   5.361
_cell_volume                     447.521
_citation_journal_id_ASTM        ZEKRDZ
_cod_data_source_file            Murakami_ZEKRDZ_1984_1907.cif
_cod_data_source_block           Mg1O3Si1
_cod_original_cell_volume        447.5214
_cod_original_formula_sum        'Mg1 O3 Si1'
_cod_database_code               8104506
Crystal Structure of Di-Strontium Boro-Aluminate, 2(SrO)~2~⋅Al~2~O~3~⋅B~2~O~3~
Nagai, T.; Ihara, M.; Journal of the Ceramic Association, Japan 80 (1972) 432–437; doi:10.2109/jcersj1950.80.927_432

data_1542236
_publ_section_title
;
 Crystal Structure of Di-Strontium Boro-Aluminate,
 2(SrO)~2~&#x22C5;Al~2~O~3~&#x22C5;B~2~O~3~
;
_journal_issue                   927
_journal_name_full               'Journal of the Ceramic Association, Japan'
_journal_page_first              432
_journal_page_last               437
_journal_paper_doi               10.2109/jcersj1950.80.927_432
_journal_volume                  80
_journal_year                    1972
_chemical_formula_sum            'Al B O4 Sr'
_chemical_name_systematic        'Sr B Al O4'
_space_group_IT_number           56
_symmetry_space_group_name_Hall  '-P 2ab 2ac'
_symmetry_space_group_name_H-M   'P c c n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   15.17(4)
_cell_length_b                   8.86(3)
_cell_length_c                   5.48(2)
_cell_volume                     736.546
_citation_journal_id_ASTM        YGKSA4
_cod_data_source_file            Nagai_YGKSA4_1972_362.cif
_cod_data_source_block           Al1B1O4Sr1
_cod_original_formula_sum        'Al1 B1 O4 Sr1'
_cod_database_code               1542236
Crystallographic studies and structural systematics of the C2/c alkali metal metavanadates
Ng, H.N.; Calvo, C.; Idler, K.L.; Journal of Solid State Chemistry 27 (1979) 357–366; doi:

data_1542237
_publ_section_title
;
 Crystallographic studies and structural systematics of the C2/c alkali
 metal metavanadates
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              357
_journal_page_last               366
_journal_volume                  27
_journal_year                    1979
_chemical_formula_sum            'Li0.5 Na0.5 O3 V'
_chemical_name_systematic        'Na0.5 Li0.5 V O3'
_space_group_IT_number           15
_symmetry_space_group_name_Hall  '-C 2yc'
_symmetry_space_group_name_H-M   'C 1 2/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 100.13
_cell_angle_gamma                90
_cell_formula_units_Z            8
_cell_length_a                   10.179
_cell_length_b                   9.061
_cell_length_c                   5.845
_cell_volume                     530.692
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Ng_JSSCBI_1979_1476.cif
_cod_data_source_block           Li0.5Na0.5O3V1
_cod_original_cell_volume        530.6917
_cod_original_formula_sum        'Li0.5 Na0.5 O3 V1'
_cod_database_code               1542237
Crystallographic studies of olivine-related sarcopside-type solutions
Nord, A.G.; Zeitschrift fuer Kristallographie (149,1979-) 166 (1984) 159–176; doi:

data_8104507
_publ_section_title
;
 Crystallographic studies of olivine-related sarcopside-type solutions
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              159
_journal_page_last               176
_journal_volume                  166
_journal_year                    1984
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Co1.05 Ni1.95 O8 P2'
_chemical_name_systematic        '(Ni0.65 Co0.35)3 (P O4)2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 91.09
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.185
_cell_length_b                   4.713
_cell_length_c                   5.865
_cell_volume                     281.480
_citation_journal_id_ASTM        ZEKRDZ
_database_code_amcsd             0020846
_exptl_crystal_density_diffrn    4.321
_cod_data_source_file            Nord_ZEKRDZ_1984_1901.cif
_cod_data_source_block           Co1.05Ni1.95O8P2
_cod_original_cell_volume        281.4802
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_database_code               8104507
_amcsd_formula_title             (Ni0.65Co0.35)3(PO4)2
Crystallographic studies of olivine-related sarcopside-type solutions
Nord, A.G.; Zeitschrift fuer Kristallographie (149,1979-) 166 (1984) 159–176; doi:

data_8104508
_publ_section_title
;
 Crystallographic studies of olivine-related sarcopside-type solutions
;
_journal_name_full
'Zeitschrift fuer Kristallographie (149,1979-)'
_journal_page_first              159
_journal_page_last               176
_journal_volume                  166
_journal_year                    1984
_chemical_compound_source        Synthetic
_chemical_formula_sum            'Co1.95 Ni1.05 O8 P2'
_chemical_name_systematic        '(Ni0.35 Co0.65)3 (P O4)2'
_space_group_IT_number           14
_symmetry_space_group_name_Hall  '-P 2yab'
_symmetry_space_group_name_H-M   'P 1 21/a 1'
_cell_angle_alpha                90
_cell_angle_beta                 91.07
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   10.247
_cell_length_b                   4.728
_cell_length_c                   5.889
_cell_volume                     285.259
_citation_journal_id_ASTM        ZEKRDZ
_database_code_amcsd             0020844
_exptl_crystal_density_diffrn    4.267
_cod_data_source_file            Nord_ZEKRDZ_1984_1902.cif
_cod_data_source_block           Co1.95Ni1.05O8P2
_cod_original_cell_volume        285.2594
_cod_original_sg_symbol_Hall     '-P 2ybc (z,y,-x)'
_cod_database_code               8104508
_amcsd_formula_title             (Ni0.35Co0.65)3(PO4)2